Synthesis and characterization of dendritic compounds containing nitrogen: monomer precursors in the construction of biomimetic membranes

In this article, we synthesized a novel dendritic 2-oxazoline, 2-(3,4,5-tris(4-dodecyloxybenzyloxy)phenyl)-4,5-dihydro-1,3-oxazole), and its amide precursor N-(2-hydroxyethyl)-3,4,5-tris(4-dodecyloxybenzyloxy)benzamide. Of the distinct synthetic routes explored, it was established that the direct amidation of esters with sodium methoxide followed by the dehydrative cyclisation with 2,3-dichloro-5,6-dicyano-1,4-benzoquinone as oxidizing agent and triphenylphosphine was the most efficient route to synthesize the dendritic 2-oxazoline. Besides, N-(2-hydroxyethyl)-3,4,5-tris(4-dodecyloxybenzyloxy)benzamide exhibited a monotropic columnar mesophase, whilst the dendritic 2-oxazoline does not exhibited a liquid crystalline mesophase. At the end, the first attempts to polymerize the 2-oxazoline monomer via cationic ring opening polymerization showed promising results. Therefore, the dendritic 2-oxazoline could be used as a mesogenic monomer in the synthesis of side-chain liquid-crystalline polyoxazolines that might self-assembly into columnar structures.

www.nature.com/scientificreports/ 2-oxazolines and the subsequent self-organisation of the dendronized poly(ethyleneimine)s into LC phases via self-assembly process [24][25][26][27] . Furthermore, Kim and co-workers reported the synthesis of a family of side-chain liquid-crystalline poly(2oxazoline)s with different contents of cyanobiphenyl-based mesogenic groups 28 . Moreover, they grafted distinct mesogens that differ in the methylene units of the spacer length (2, 4, 6 and 10 methylene units, respectively) to a partially hydrolysed poly(2-methyl-2-oxazoline) via Steglich esterification. They proved that at least a modification degree equal to 27% of cyanobiphenyl mesogenic group is required in the resulting poly(2-oxazoline)s to detect a liquid-crystalline mesophase by DSC (differential scanning calorimetry) or POM (polarized optical microscopy). Furthermore, the LC phase range of the poly(2-oxazoline)s, which exhibit smectic or nematic LC textures, is correlated with the length of the spacer moiety of the mesogen.
In the last decades, our research group has focused on the design and synthesis of dendronized liquidcrystalline polyethers and polyamines by grafting dendritic side groups into these polymers, which induce their self-assembly into columnar structures, thus resulting in the formation of an inner channel, which contains polar ether or amine linkages, which allow it to work as an ion channel [29][30][31] . Membranes prepared using the previously synthesized low molecular weight side-chain liquid-crystalline polyamines exhibited a remarkable proton transport, despite their poor mechanical properties and brittleness 32,33 . To minimize these drawbacks, in this paper the synthesis of higher molecular weight side-chain liquid crystalline polyamines was tackled by the polymerization of dendritic monomers. It must be mentioned that the synthesis and characterization of a dendritic liquid-crystalline aziridine was reported by us 34 , which exhibited a monotropic columnar LC phase on cooling. Even so, attempts to polymerize it did not provide satisfactory results 34 .
Thus, in this work, we describe the synthesis and characterization of a novel dendritic 2-oxazoline monomer 2-(3,4,5-tris(4-dodecyloxybenzyloxy)phenyl)-4,5-dihydro-1,3-oxazole) (TAPOx) and its amide precursor N-(2-hydroxyethyl)-3,4,5-tris (4-dodecyloxybenzyloxy)benzamide (TAPAm). The 2-oxazoline monomer can be subsequently polymerized in a controlled manner taking advantage of the "living" character of CROP of this type of monomers to obtain side-chain liquid-crystalline acyl-substituted poly(ethyleneimine)s, that can be a promising candidate in the preparation of membranes that allow the transport of cations thanks to the presence of nitrogen atoms in their inner channel. Moreover, the nature of the CROP would let us to obtain high molecular weight SCLCPs, which will enable the preparation of membranes that should exhibit improved mechanical properties than the cation exchanges membranes tested in polymer electrolyte fuel cells with the previously synthesized side-chain liquid-crystalline polyethers and polyamines.

Synthesis of N-(2-hydroxyethyl)-3,4,5-tris(4-dodecyloxybenzyloxy)benzamide
(TA-PAm). Direct amidation method using EDC as coupling agent. In a round-bottomed flask, 0.50 g of TAPAc (0.50 mmol) were dissolved into 10 mL of chloroform. The solution was stirred at 0 °C in an ice-water bath for 15 min. Then, DMAP (49.2 mg, 0.40 mmol) was added, and the solution was kept under stirring at 0 °C during 15 min more. After that, EDC (97.3 mg, 0.50 mmol) was added, leaving the magnetic stirring for additionally 15 min at the same temperature. At this moment, ethanolamine (0.09 mL, 1.49 mmol) was added dropwise. When the addition of ethanolamine was completed, the reaction mixture was warmed to room temperature and kept under stirring. The conversion of TAPAc was monitored by TLC using n-hexane/ethyl acetate as mixture of eluents (1:2). After complete conversion of TAPAc was observed by TLC (27 h), the crude mixture was first extracted twice with water and then once with brine. The organic layer was dried over anhydrous MgSO 4 and vacuum evaporated. Finally, the obtained solid was purified by flash column chromatography (gradient of nhexane/ethyl acetate as mixture of eluents; starting proportion = 2:1), obtaining pure TAPAm as a white powder (212.5 mg, 42%). Direct amidation of TAPEs with ethanolamine. In a pear-shaped flask, 1.00 g of TAPEs (0.99 mmol) was dissolved in ethanolamine (1.98 g, 33.07 mmol). The crude of the reaction, which was monitored by TLC (n-hexane/ethyl acetate (1:2) as mixture of eluents), was vigorously stirred under reflux at 140 °C. After total conversion of TAPEs (15 h), the black solution was cooled to RT and 10 mL of CHCl 3 were added. The organic solution was extracted three times with water and then once more with brine. After that, the organic layer was dried over anhydrous MgSO 4 and vacuum evaporated. Finally, the product was recrystallized twice with ethanol, obtaining 456.6 mg of TAPAm (43%).

Preliminary polymerization studies. Bulk polymerization of TAPOx. In a previously flame-dried
Schlenk tube, 505.0 mg of TAPOx monomer (0.49 mmol) were added. Then, the tube was immersed into a preheated oil bath at 130 °C, where TAPOx was stirred during 15 min under argon flow conditions. After that, 1% mol of methyl tosylate (0.91 mg, 4.9 · 10 -3 mmol) were added and the reaction mixture was kept under argon until a complete conversion of TAPOx was detected by 1 H NMR. At this point, an excess of dodecylamine (0.50 mL, 2.17 mmol) was added as terminating agent, maintaining the same temperature for 24 h, when the crude mixture was cooled to room temperature. Finally, the resulting mixture was dissolved in THF and the polyoxazoline was isolated by precipitation twice into cold methanol, obtaining 312.0 mg of a beige solid (62%).
Characterization. Thermogravimetric analysis (TGA). Thermal stability studies were carried out in ALU OXIDE crucibles of 70 µL (ME-24123) with a Mettler Toledo TGA2 thermobalance. All samples, weighing around 6-8 mg, were heated between 30 and 600 °C at a heating rate of 10 °C/min in N 2 atmosphere with a flow rate of 50 cm 3 /min. The equipment was previously calibrated with indium (156.6 °C) and aluminium (660.3 °C) pearls.
Differential scanning calorimetry (DSC). Calorimetric analyses were carried out on a Mettler DSC-821 instruments calibrated using indium (156.6 °C) and zinc (419.6 °C) pearls. Samples were placed in an aluminum standard crucible of 40 µL with pierced lids (between 4 -6 mg of sample), which were analysed in N 2 atmosphere (gas flow rate of 50 cm 3 /min). Heating and cooling rate of 10 °C/min has been always employed.
Polarized optical microscopy (POM). LC mesophases were investigated by polarised optical microscopy (POM). The textures of the samples were observed with an Anxiolab Zeiss optical microscope equipped with a Linkam TP92 hot stage.
Nuclear magnetic resonance (NMR) spectroscopy. All synthesized compounds were characterized by 1 H NMR and 13 C NMR spectra, which were recorded in deuterated chloroform (CDCl 3 ) with a Bruker Avance Neo 400 MHz spectrometer ( 1 H-400 MHz; 13 C-100.4 MHz) at room temperature. The chemical shifts were given in parts per million (ppm) from TMS (Tetramethylsilane) in 1 H NMR spectra, while the central peak of the solvent was taken as reference in the case of 13 C NMR spectra.
Fourier transform infrared (FT-IR) spectroscopy. FT-IR spectra were recorded on an FT/IR-6700 spectrophotometer from JASCO in the wavelength range of 4000-400 cm −1 with a resolution of 4 cm −1 in the absorbance mode. This device is equipped with an attenuated total reflection accessory (ATR) with thermal control and a diamond crystal (Golden Gate heated single reflection diamond ATR from Specac-Teknokroma). The spectra were recorded at room temperature from the solid-state pure compounds.
X-ray diffraction (XRD). X-ray diffraction measurements (XRD) were made using a Bruker-AXS D8-Advance diffractometer with vertical θ-θ goniometer, incident-and diffracted-beam Soller slits of 2.5°, a fixed 0.5° receiving slit and an air-scattering knife on the sample surface. The angular 2θ range was between 2 and 40°. The data were collected with an angular step of 0.02° at a step/time of 0.5 s. Cukα radiation was obtained from a copper X-ray tube operated at 40 kV and 40 mA. Diffracted X-rays were detected with a PSD detector LynxEye-XE-T with an opening angle of 2.9°. The sample was placed inside an MTC-LOWTEMP chamber for in-situ temperature analysis.

Results and discussion
The main goal of this work was the synthesis of a dendronized 2-oxazoline monomer bearing the tapered 3,4,5-tris[4-(n-dodecan-1-yloxy)benzyloxy)benzoate group, which will allow us to prepare LC poly(2-oxazoline) s by living CROP. Moreover, the thermal and mesomorphic characterization of the new mesogenic compounds was performed to determine their LC mesophases.
The synthetic pathway of both dendrons was described in previous studies 31 and in the experimental section of this paper. Their chemical structure is depicted in Fig. 1.
Regarding the first step, the esterification of carboxylic acids using a carbodiimide as a promoter along with dimethylaminopyridine (DMAP) to activate an acid and favour the ester formation is one of the most common esterification methods employed due to the high number of advantages that this reaction shows: high versatility, mild conditions are usually required for the reaction to proceed (room temperature), which also facilitates its use with different types of substrates 37 . Moreover, it allows the obtention of esters from tertiary alcohols because the steric impediments do not affect this type of esterification. It was mentioned before that our group reported the chemical modification of polyethers and polyamines with the dendron 3,4,5-tris[p-(n-dodecan-1-yloxy)benzyloxy]benzoic acid (TAPAc) by means of Steglich esterification, obtaining side-chain liquid crystalline polyethers and polyamines [30][31][32] . The promoter that we used in all these studies was N,N'-dicyclohexylcarbodiimide (DCC) 31 .
Despite the advantages of Steglich esterification, this reaction presents some drawbacks: stoichiometric amounts or more of the carbodiimide are required, the yields are not always high and undesired N-acylureas are occasionally formed. These disadvantages may be minimized by the addition of strong acids like p-toluenesulfonic acid 38 , N-hydroxy derivatives 39 or tertiary amines 40 , which suppress the formation of N-acylurea and favour the formation of the corresponding ester.
In this direction, the amidation of amines instead of alcohols to the corresponding amides took place with DCC as coupling agent following the same mechanism because amines present a more nucleophilic character. Therefore, the amidation of TAPAc with ethanolamine using the same conditions reported previously was carried out (Fig. S1 in Supplementary information). Although ethanolamine also contains a hydroxyl group, the amidation reaction will be favoured due to the chemoselectivity of the amine group present in ethanolamine versus the hydroxyl group. The dendronized amide was obtained in our case, even though a large amount of the N-acylurea side product was found mixed with TAPAm. Nonetheless, the complete removal of the dicyclohexylurea (DCU) was not possible by the purification methods employed in the work-up process of the crude mixture: filtration or flash column chromatography; obtaining always a highly impurified product.
To avoid this problem, DCC was replaced by a water soluble carbodiimide, 1-ethyl-3-(3-dimethylaminopropyl)carbodiimide (EDC). Despite EDC is an expensive reagent, the formed N-acylurea can be easily removed by aqueous extraction 39,41,42 . Besides, it was observed that the formation of the amide took place faster when EDC was used as coupling agent compared with the reaction using DCC (27 h vs. 4 days, respectively). Nonetheless, it was still necessary to purify the crude mixture by flash column chromatography.
Although amides can be obtained from carboxylic acids, we can take advantage of the greater reactivity of the ester group present in TAPEs to synthesize TAPAm 43,44 . In this way, Percec and co-workers reported a simple method for the amidation of dendronized esters into the corresponding amides by using a large excess of ethanolamine with yields higher than 80% 26,45 . So, the direct amidation of TAPEs with ethanolamine was also explored following the conditions reported by Percec group to increase the yield in the synthesis of TAPAm. Nevertheless, lower yields were obtained in our case (43%).
On the other hand, the addition of a catalyst facilitates the formation of amides from the corresponding esters under mild conditions with excellent yields. Different types of catalyst have been reported in literature, which exhibited an improved efficiency in the formation of amides: inorganic catalysts such as Sb(OEt) 3 46 or Zr(O t Bu) 4 -HOAt) 47 ; or organic catalysts, including N-heterocyclic carbine 48 , DBU 49 and triazabicyclo [4.4.0]dec-5-ene 50 . Furthermore, Yang and co-workers showed that the combination of different catalysts (1,2,4-triazole and DBU) accelerates the ester conversion to generate the corresponding amides at room temperature in high yields 51 . However, the preparation of many of these catalysts is quite complex, which implies that the catalytic activity of simpler and cheaper compounds is investigated. In this sense, sodium methoxide (NaOMe) is a wellknown commercial compound that is widely used as catalyst in the production of biodiesel by transesterification of triglycerides with methanol 52 . When Ohshima et al. used catalytic amounts of sodium methoxide (≤ 10%) in the direct amidation of esters, they observed that the addition of this non-toxic catalyst results in the obtention www.nature.com/scientificreports/ of the corresponding amides under mild conditions, although this reaction requires the use of inert atmosphere to suppress the saponification of the starting esters 53 . According to that, this procedure was followed in the amidation of TAPEs (Fig. 2). In our case, the addition of 10% mol of NaOMe not only simplified the work-up process of TAPAm, since flash column chromatography was replaced by a recrystallization in EtOH, but also caused an increase of more than double of the yield of the reaction with respect to the attempts reported before (92%). Table 1 shows the different precursors, the solvent and the reaction conditions used in the chemical reactions tested in the synthesis of TAPAm, together with the obtained results.
To confirm its chemical structure, dendronized TAPAm precursor was characterized by NMR and FT-IR spectroscopy. Figure 3 shows its 1 H NMR spectrum, which was performed using CDCl 3 as solvent. The aromatic region shows five signals at 7.23, 7.16, 6.98, 6.80 and 6.67 ppm. In comparison with previously reported characterization of methyl 3,4,5-tris[p-(n-dodecan-1-yloxy) benzyloxy] benzoate 54 , the signals at 7.23 and 7.16 ppm (6 H) can be assigned to the protons in ortho position to -CH 2 O-of lateral and central benzylic units, respectively. The signal at 6.98 ppm (2 H) corresponds to the protons of the benzoate group linked to the amide, whose multiplicity appears as a singlet. The other two signals at 6.80 and 6.67 ppm correspond to the protons in metha position to -CH 2 O-of the lateral and central benzylic units, respectively. Furthermore, a triplet at 6.47 ppm corresponds to the proton of the amide group (-NH-), which is coupled to the neighbouring methylene as observed in the recorded 2D NMR spectra (COSY and HSQC NMR spectra; Figs. S2 and S3 in Supplementary information). The two signals centred at 4.93 and 4.90 ppm are assigned to the benzylic methylenes of the dodecyloxybenzyloxy substituents. Moving upfield in the spectrum, two triplets centred at 3.86 and 3.83 ppm are attributed to methylene attached to the oxygen in the long alkyl chains in lateral and central benzylic units, respectively. As we move to lower chemical shifts, the presence of two characteristic signals at 3.73 and 3.50 ppm confirm that the amidation reaction took place because they are assigned to the N-(hydroxyethyl) moiety. Particularly, the triplet at 3.73 is assigned to the methylenic protons next to the hydroxylic group, while the signal at 3.50 ppm corresponds to the methylene unit contiguous to the amide group, since these protons are coupled to neighbouring methylene group and -NH proton as confirmed by 2D NMR experiments (COSY and HSQC; Figs. S2 and S3 in Supplementary information). Finally, the signals at 1.70, 1.37, 1.20 and 0.81 ppm of the high-field region can be assigned to the protons of the alkyl long chains of the dendron. Figure 4 shows the 13       Due to the versatility of the oxazoline functional group, considerable efforts have been made to develop a broad scope of synthetic routes starting from esters 55,56 , nitriles 57 , carboxylic acids 58,59 and N-(hydroxyethyl) amides 3,60,61 . From all of them, one of the most simple and well-known process is to convert the hydroxyl group of the N-(2-hydroxyethyl)amides into a good leaving group using thionyl chloride (SOCl 2 ), followed by a basic treatment with NaHCO 3 to isolate the 2-oxazoline derived ring 62 . Unfortunately, from what was observed when this reaction was carried out with TAPAm, the generated HCl in the reaction medium induced the cleavage of the ether benzylic moieties present in TAPAm. To suppress this side reaction, an excess of a non-nucleophilic base (DBU) was added before the addition of thionyl chloride to act as scavenger of the in-situ generated hydrochloric acid during the reaction as Šakalytė and co-workers did 31 . Nonetheless, the formation of TAPOx was not detected in the crude mixture while TAPAm was being consumed.
Thus, alternative reagents that favour the dehydrative cyclisation of amides should be considered. We selected the methodology reported by Xu and co-workers, who described a facile and rapid procedure for the synthesis of 2-oxazolines using PPh 3 -DDQ as oxidizing agent 63 . Among the advantages of this reaction, the authors highlighted its versatility (because it works well with distinct solvents such as DCM, 1,4-dioxane, THF, toluene), the mild reaction conditions (it takes place at room temperature) combined with the high yields of 2-oxazoline. Therefore, the synthesis of TAPOx was attempted using the PPh 3 -DDQ system (Fig. 5) and DCM as solvent. As Xu and co-workers previously demonstrated with various esters, we detected a complete conversion of the amide (TAPAm) by TLC after 20 min and TAPOx was isolated from the crude mixture by flash column chromatography with a high yield (85%).
To validate the chemical structure of TAPOx, the obtained product was characterized by NMR and FT-IR spectroscopy. Figures 6 and 7 show the 1 H NMR and 13 C NMR spectra of TAPOx respectively, which were recorded using deuterated chloroform as solvent.
Starting with the downfield region in 1 H NMR spectrum, the peaks between 7.25 and 6.67 ppm are assigned to the aromatic protons of the molecule. The two singlets that appear between 4.96 and 4.91 ppm are assigned to  Moreover, these assignments are in agreement with the characterization of 2-oxazoline monomers previously described by Percec and co-workers 26,45 . Furthermore, the two triplets centred at 3.89 and 3.84 ppm are attributed to methylene attached to the oxygen in long alkyl chains in lateral and central benzylic units, respectively. In the same manner than in the precursor TAPAm, signals between 1.70 and 0.81 ppm are attributed to the alkyl long chains of the dendron. Related to 13 C NMR, the carbon signal attributed to the -C=N-of the oxazoline ring appears at 164.7 ppm. The signals between 159.1 and 107.9 ppm are attributed to the aromatic carbons of the dendronized 2-oxazoline monomer. Is remarkable that the carbon of the aromatic ring linked to the oxazoline cycle appears slightly upfield in the spectrum compared to TAPAm precursor (122.9 ppm in front of the 129.5 ppm value observed in TAPAm). Same as TAPAm, the signals of the carbons that constitute the long alkyl chains appear at the expected region between 32.1 and 14.3 ppm (carbons labelled as a-e). The signals at 67.9 and 55.0 ppm are assigned to both methylene units of the 2-oxazoline ring, being the signal that appears at 67.9 ppm the one that corresponds to the methylene next to the oxygen, while the signal at 55.0 ppm is attributed to the methylene unit bonded to the nitrogen of the cycle. HSQC and HMBC NMR spectra allowed us to confirm the assignment of the characteristic signals of the 2-oxazoline ring (Figs. S5 and S6 in Supplementary information). Besides, the assignment agrees with the elucidation described in previous studies by Percec and co-workers 26,45 .
Moreover, the characteristic functional groups found in the chemical structure of TAPOx were characterized by FT-IR spectroscopy. In its FT-IR spectrum, no bands were observed above 3000 cm −1 and a new band attributed to the C=N stretching appears at 1643 cm −1 , which is characteristic of the 2-oxazoline ring and confirms that the dehydrative cyclisation of N-(2-hydroxyethyl)-3,4,5-tris(4-dodecyloxybenzyloxy)benzamide was achieved 64 .
Finally, the direct synthesis of TAPOx from methyl 3,4,5-tris[p-(n-dodecan-1-yloxy)benzyloxy]benzoate (TAPEs) using lanthanide salts as catalyst was explored. The main advantage of this synthetic route is that only involves a single-step reaction as demonstrated by Zhou et al. 55 . In their work, the authors developed a simple and efficient method for the amidation of different carboxylic esters taking advantage of distinct inorganic catalyst (LaCl 3 , LaTf 3 and SmCl 3 ) obtaining 2-oxazolines in good yield when the reaction was performed under reflux of toluene. According to that, we carried out the one-pot synthesis of TAPOx from the starting ester dendron (TAPEs) using the conditions reported by Zhou and co-workers. In our case, different catalytic amounts of LaCl 3 (5, 10, 20% mol respect to TAPEs) and LaTf 3 (10% mol respect to TAPEs) were tested as catalyst. Nevertheless, the formation of 2-oxazoline compound was never detected in the reaction medium even though the formation of the amide (TAPAm) was observed when lanthanum triflate was employed. These observations agree with the results presented by Morimoto and co-workers, in which they reported the amidation of esters using 5% mol of LaTf 3 in mild conditions with good yields (≥ 80%) 65 . However, we could not isolate the TAPAm fraction from the crude mixture even by flash column chromatography due to its complexity and the low amount of TAPAm that it presented. www.nature.com/scientificreports/ To summarize the reactions that were carried out in the synthesis of TAPOx, Table 2 presents the starting materials, the solvent and the reaction conditions employed in all the reactions performed. Furthermore, the obtained yield and general remarks have been also shown.
At the end, Fig. 8 outlined all the synthetic routes that we had explored to obtain TAPOx monomer.
Thermal and mesomorphic characterization of TAPAm and TAPOx. Thermal and mesomorphic characterization of TAPAm and TAPOx was performed by DSC, TGA, POM and XRD experiments. DSC study of TAPAm is depicted in Fig. 9. First and second heating scans are shown as well as the first cooling scan. The  www.nature.com/scientificreports/ first heating scan shows a broad endotherm at 84 °C, followed by a second sharper endotherm at 101 °C; finally, a small endotherm is shown at 118 °C. On cooling scan, we only observe an exotherm centred at about 83 °C. At second heating scan, we are able only to see two endotherms, the first one centred at 101 °C and the second one at 118 °C. As we could observe, after the clearing of the substrate the first endotherm was no longer observed, showing only these two peaks which are compatible with the occurrence of a mesophase in the range of temperatures from 101 to 118 °C. Table 3 shows the associated enthalpies for each phase transition and clearing temperature for TAPAm on first and second heating scans. Based on DSC and XRD experiments (Fig. 10), we observed a metastable crystalline phase below first endotherm on first heating, since this phase was not observed at the second heating. On the other hand, we envisioned a highly ordered columnar phase between 84 and 101 °C at first heating. POM observation, in this range of temperatures, put into evidence a pseudo-focal conic fan-shaped texture (Fig. 11). XRD pattern recorded at 90 °C (Fig. 10b) shows three main peaks centred at 2θ = 2.4° (d = 36 Å), 4.6° (d = 19 Å), 6.2° (d = 14 Å) and an unsymmetrical broad halo at 2θ = 20° (d = 4 Å approximately) showing shoulders. The lower spacing observed in the XRD pattern should correspond to the planar distance between dendrons and the higher spacing might correspond to the lateral distance between columns. It is noteworthy that for the second heating only this phase was observed below the endotherm centred at 101 °C.
For the range of temperature between 101 and 118 °C, we observed the presence of a mesophase. This was confirmed by XRD experiments, with a pattern recorded at 110 °C (Fig. 10c,e); we saw four main peaks centered at 2θ = 2.6° (d = 34 Å), 3.9° (d = 22 Å), 4.3° (d = 20 Å), 4.9° (d = 18 Å) and a symmetrical broad halo at 2θ = 20° (d = 4 Å approximately). Same as before, the lower spacing can be attributed to the distance between dendrons and the higher one to the lateral distance between columns. In this case, the phase observed is quite disordered, as we could inferred by DSC, where the enthalpy of the endotherm was only 0.8 kJ/mol (Table 3). Furthermore, on second heating we observed the same behaviour as first heating in the range of temperatures from 101 to 118 °C. It is remarkable that on cooling from the melt state we did not observe the formation of this phase by DSC nor POM. Therefore, it is suggested that TAPAm should present a monotropic columnar mesophase in the range of temperature from 101 to 118 °C.
Calorimetric study by DSC of TAPOx is depicted in Fig. 12, showing first and second heating and cooling scans. On heating we observe one endotherm centered at 89 °C for the first heating and 86 °C for the second heating, which can be attributed to the melting of TAPOx, meanwhile on cooling we observe a peak centered at 73 °C, which can be assigned to the crystallization of TAPOx. According to POM experiments, on heating we did not observe a mesophase below melting point and an isotropic liquid was observed above the endotherm. Moreover, on cooling we did not notice the presence of a mesophase from the melt state. This behaviour was also confirmed by XRD experiments, showing a crystalline phase below the melting point and an isotropic liquid above the  www.nature.com/scientificreports/ endotherm (Fig. S7). Therefore, TAPOx shows no mesomorphic behaviour. Thus, it seems that the stiffness of the oxazoline ring strongly difficults the packing of tapered groups, avoiding the formation of columnar phases. Thermal stability of TAPAm and TAPOx was studied by TGA (Fig. 13). Onset of thermal weight loss (determined as the temperature corresponding to 5% mass loss) was 271 °C for TAPAm with 14% of remaining char yield at 600 °C. TAPOx is slightly more stable, with an onset of the thermal weight loss of 285 °C and a similar char yield at 600 °C (15%) compared with its amide precursor. In the case of TAPEs, it presents the higher onset of thermal weight loss of the 3 dendronized compounds: 291 °C, but the smallest remaining char yield (12%). Besides, the thermal degradation of these three dendronized compounds showed a two-step weight loss, as confirmed by DGTA curves (Fig. S8). The presence of a hydroxyl group in TAPAm chemical structure can lead to  www.nature.com/scientificreports/ an easy dehydration that could induce the thermal degradation of TAPAm at a lower temperature than TAPOx and TAPEs, which DTGA curve showed the same trend.
Preliminary polymerization study. As aforementioned, it is described that 2-substituted-2-oxazolines polymerize by living cationic ring opening polymerization (CROP). Many procedures to polymerize these compounds can be founded in literature, i.e. Percec and co-workers described the polymerization of 2-[3,4-bis(nalkan-1-yloxy)phenyl]-2-oxazolines using o-dichlorobenzene as a solvent at 110 °C and bulk polymerization at 160 °C, with methyl triflate (MeOTf) as an initiator 26 . Apart from MeOTf, a wide variety of initiators have been used, such as sulfonate esters, Lewis acids and alkyl halides among others 10 . Furthermore, several terminating agents have been employed in this type of polymerizations, such as primary, secondary and aromatic amines, hydroxide salts and alcohols, among others 3 .
Herein, we describe a preliminary study of polymerization of TAPOx. All the conditions tested in each polymerization of TAPOx are summarized in Table 4. On our first attempt, we try to synthetize our polymer using methyl tosylate (MeOTs) as an initiator and toluene as a solvent under reflux conditions. We monitored the reaction by 1 H NMR; nevertheless, after 12 days of reaction the product was not noticed, and only unreacted monomer was observed at the reaction medium. On a second attempt, we follow the procedure described by Pásztói et al. 66 , where benzotrifluoride was used as an environmentally less harmful solvent to polymerize 2-ethyl-2-oxazoline at 100 °C using MeOTs as an initiator. Unfortunately, following the same trend as the first attempt, the polymer was not detected after 10 days of reaction and only unreacted TAPOx was present at the reaction medium.  www.nature.com/scientificreports/ Therefore, we decided to carry out a bulk polymerization of TAPOx at 130 °C using MeOTs as an initiator. In this case, we could confirm the total conversion of the monomer through 1 H NMR analysis (Fig. 14a) and 13 C NMR (Fig. 14b) experiments. Regarding 1 H NMR analysis, the characteristic signals corresponding to both methylenes in the oxazoline ring at 4.34 and 3.97 ppm (see Fig. 6) disappear and a broad signal corresponding to the main chain of polyoxazoline appears centred at 3.67 ppm. Furthermore, according to 13 C NMR experiments, full conversion of TAPOx was also confirmed, since the signal corresponding to the methylene contiguous to nitrogen inside the oxazoline ring, at 55.0 ppm (see Fig. 7), also disappeared. Despite the full conversion of the monomer was confirmed by NMR, the yield of the polymerization after work-up was only 62%. This fact indicates us that we must optimize the purification process. Besides, based on the relationship between the signals of the terminating agent added (dodecylamine) and the polymer in 1 H NMR, we found that only oligomers were synthetized; in fact, pentamers were obtained.
As a complementary analysis, we decided to observe the synthesized oligomers by polarized optical microscopy in order to see whether it presents a mesophase. We found that, on heating, a mesophase was noticed, actually, an homeotropic texture was observed.
It is clear that, the polymerization of TAPOx deserves a deeper study, in order to find the conditions to get a columnar polyoxazolines of quite high molecular weight. This study is in progress and will be the subject of a forthcoming paper.

Entry
Initiator (% mol)/terminating agent Solvent Reaction conditions Comments/yield (%)  Figure 14. Zooms of the NMR spectra of the polyoxazoline derived from TAPOx: (a) 1 H NMR spectrum between 2.5 and 5.5 ppm (signals labelled in red); and (b) 13 C NMR spectrum between 50 and 80 ppm (signals labelled in blue). www.nature.com/scientificreports/ dehydrative cyclisation of the amide using PPh 3 -DDQ system as oxidizing agent. Although the corresponding 2-oxazoline derived monomer was purified by flash column chromatography, TAPOx was also obtained with a good yield (85%). Thermal and mesomorphic studies showed that a monotropic columnar mesophase was observed on heating for TAPAm in the range of temperatures from 101 to 118 °C, meanwhile any liquid crystalline texture was detected in the case of TAPOx.
Furthermore, a preliminary research of the cationic ring opening polymerization of TAPOx was carried out, from which it was deduced that a profound investigation should be addressed to find the optimal conditions to get columnar polyoxazolines with high molecular weight.